LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS


 Marlene Walton
 2 years ago
 Views:
Transcription
1 XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds it all together. A corresponding and related lamination theory for the strength of laminates would be equally important and useful. It would complete the understanding of the behavior of fiber composite materials in its most important and prime form of usage, laminates. This research report extends the technical program established in Ref. [1]. In that work Christenen and Lonkar [1] developed failure criteria that were mainly intended for quasiisotropic fiber composite laminates. This work develops the much broader and much more generally useful failure criteria for wide classes of orthotropic fiber composite laminates. The quasiisotropic laminates case is important because it is one limiting case of fiber composite laminations. The other limiting case is the unidirectional form itself. The class of orthotropy supplies the general and inclusive bridge of cases in between and including these two limiting cases. General cases such as these have been treated in the large and highly publicized composites failure program of Hinton and Kaddour [2]. The end result of that program served more to show the utter and unrelenting complexity of the overall problem rather than providing any unified and directly applicable results. The following work will begin by recalling some previous results from Ref. [1] and then pursuing a very large scale extension of the method. This will allow the treatment of the general case of orthotropic laminates where the degree of anisotropy in the plane of the laminate can be arbitrarily specified as necessary for a very wide range of layup patterns and problem specifications. At the lamina level the fiber composites form will be taken as highly anisotropic, appropriate to very high stiffness and high strength fibers (typified by carbon fibers) in a polymeric matrix. It will be found that the failure criteria for the general orthotropic laminate is completely calibrated by only two fiber dominated failure properties at the unidirectional lamina or the tow level of the fibermatrix
2 system. Calibrating the failure theory for general orthotropic laminates by use of only two failure properties certainly would have been thought to be impossible. This seemingly intractable problem will be solved here, removing a large obstacle to meaningful fiber composites applications. The case of unidirectional fiber composites failure was treated in Ref. [3]. As already discussed, the complementary case of the failure of quasiisotropic laminates was treated in Ref. [1]. Associated with these two works, then the present work completes the longstanding task by rigorously treating the failure of a very wide class of orthotropic laminates. This new work on composites failure could equally well be presented in a mechanics oriented materials journal or a composite materials journal. The application is to composites but the methodology is totally mechanics based. This development would not be possible were it not for the insight and avenues of approach opened up by only the mechanics discipline. The usual composites failure approach zeroes in on one particular failure mechanism and treats that in some, usually great detail. The mechanics approach used here is much broader and more inclusive, but not at the expense of rigor. The present approach will be found to be satisfyingly rigorous and general The primary reason for conducting this research and writing this paper is to provide a viable tool for use with computational mechanics. Composites research sources seem to be preoccupied with other matters and not interested in pursuing the general failure problem. Perhaps the failure problem is considered by them to be too difficult or even impossibly difficult. Nevertheless the problem desperately needs attention, solution, and subsequent application. This work accepts the challenge to produce general failure results so that computational mechanics can then take over and open up new directions for the applications of fiber composite materials. Orthotropic Laminates Failure Theory In Ref. [1] Christensen and Lonkar derived the failure criterion for quasiisotropic laminates. It was shown to have the same form as that for threedimensionally isotropic materials when in the 2D state of plane stress. It is given by 1 T 1 C σ T 1 C σ TC σ σ 11 σ 22 + σ TC σ (1)
3 where T and C are the uniaxial strengths of the laminate. Now rewrite this in slightly modified but equivalent form that will be helpful in the following orthotropic developments, as given by 1 T 1 C σ T 1 C σ σ 11 TC σ 11 TC σ 22 TC + σ 22 TC TC σ (2) In Ref. [1] the quasiisotropic form in (2) was shown to generalize to the failure criterion for orthotropic laminates in plane stress as 1 1 σ T 22 σ 22 + C 11 σ 11 C 11 2 C 22 σ 11 σ 22 C 11 T 22 C 22 + σ 22 T 22 C σ S 12 (3) where, C 11, T 22, C 22 are the tensile and compressive strengths in the 1 and 2 stress directions and S 12 is the shear strength. The orthotropic form given in Ref. [1] appears a little different from that in (3) but it is equivalent. These five calibrating strengths are directly measurable from standard, single stress component 1D tests. Form (3) is remarkably simple for the failure criterion of fully and generally orthotropic laminates. It will be developed even much further in the following derivation. For these further developments, temporarily return to the case of the quasiisotropic laminate, as treated in Ref. [1]. The failure criterion (1) only requires two strength properties to completely calibrate it. These are the uniaxial tensile and compressive strengths T and C. In a special development in Ref. [1] it was shown that the uniaxial strengths T and C for the laminate can be expressed in terms of the unidirectional fiber composites tow strengths as T = T tow 3 (4) and
4 C = C tow 3 (5) These are physically realistic approximations that apply for fiber dominated systems. The term fiber dominated means that the fibers are greatly stiffer and stronger than is the surrounding polymeric matrix phase of the composite material. In effect then the fiber phase is a completely one dimensional reinforcing agent, meaning that the fiber contribution to the stiffness and strength of the laminate is purely through its unidirectional, axial direction contribution. A slightly more complicated quasiisotropic form than (5) for the compressive strength property was derived in Ref. [1]. The simpler form (5) will be used here. It is here considered that the form in Ref. [1] is more appropriate for use with the unidirectional compressive strength being obtained from a very thin lamina form allowing the kink band mechanism of failure whereas the form (5) is more appropriate for use when the unidirectional compressive strength as determined from a monolithic type test specimen. The form (5) will be used here as being representative of the compressive strength obtained directly from the impregnated fiber tow as manufactured rather than from the further processed lamina form. Next the fiber dominated forms (4) and (5) for the quasiisotropic case will be generalized for use with the orthotropic case. This will be found to be a major and completing step forward in understanding general composites laminate strength behavior. The orthotropic laminate will be taken as the standard 0, 90, ± 45 degree layup pattern as shown in Fig. 1.
5 Fig. 1 Lamination pattern Take c 0, c 45, c 45, and c 90 as the specified volume fractions of the four lamina orientations in the orthotropic laminate. For orthotropic symmetry it is required that Thus it follows that c 45 = c 45 (6) c 0 + 2c 45 + c 90 = 1 (7) The objective here is the generalization for fiber dominated systems from the quasiisotropic case (4) and (5) to the orthotropic case. The five calibrating strengths, C 11, T 22, C 22, and S 12 will now be derived in terms of the general volume fractions c 0, c 90, and c 45 and they will be left open to later specification for particular cases. First consider the shear strength S 12. For the fiber dominated system the 0 and 90 plies make no contribution to the shear strength, only the 45 plies give shear resistance. Furthermore the shear strength must be proportional to the volume of
6 the active material in shear deformation and thus must be linearly dependent on c 45. Then take S 12 = αc 45 T tow C tow (8) where α is an unknown coefficient to be determined. The dependence shown in (8) on T tow and C tow follows from the quasiisotropic form for S from (1) as S = TC 3 = 1 3 T tow C tow 3 (9) Lastly parameter α in (8) at c 45 = ¼ then requires α = (10) to recover the form in (9). This completes the determination of orthotropic S 12. The other 4 cases for the uniaxial strengths are considerably more complex to determine. Before proceeding to the next cases it should be noted that this fiber dominated approach can give some strength properties as being zero. For example, if there were no ± 45 plies then the shear strength (8) would vanish. Of course this just would mean that the failure is totally matrix controlled and would be of very low strength capability compared with the fiber dominated and controlled failure modes. This would further mean that this would be a very poor design and should be discarded. The path to be followed for the determination of, C 11, T 22, C 22 is exactly like that of the classical lamination theory used with stiffness. But instead of stiffness, strength will be the determining factor. With stiffness the lamination theory procedure usually requires a computer to keep account of the bookkeeping for the tensor transformations. But for the fiber dominated strength problem the procedure is much simpler since the fibers are one dimensional load bearing members. In fact it is rather intriguing to watch the theory unfold and lead to surprisingly simple and clear results. First for the determination of the uniaxial strength take a unit strain in the direction. This induces a strain and consequently a fiber direction stress in the ± 45
7 lamina, for these fiber dominated lamina. Now resolve this c 45 stress into the coordinate axes directions using the tensor transformations. For no transverse stress in the laminate to exist, the 2 direction stress in the ± 45 lamina must be resisted by the 90 degree lamina. This leads to the determination of the orthotropic Poisson s ratio ν 12 as Similarly it is found that ν 12 = ν 21 = c 90 c 45 (11) c 0 c 45 (12) When c 45 = 0 then from (11) and (12) ν 12 = ν 21 = 0 as must be the case for the fiber dominated system in a crossply laminate. When c 90 = 0 in (11) then ν 12 = 1 meaning that there is no resistance to lateral strain change. Similarly when c 0 = 0 in (12). Finally the resolution of all the fiber direction stresses into the 1 direction gives the uniaxial tensile strength in that direction as Similarly it can be derived that and = c 0 + c 45c 90 c c 90 T tow (13) C 11 = c 0 + c 45c 90 c c 90 C tow (14) T 22 = c 90 + c c 45 0 c c 0 T tow (15)
8 C 22 = c 90 + c 45c 0 c c 0 C tow (16) The completing shear strength from (8) and (10) is given by S 12 = 4c 45 3 T tow C tow 3 (17) Relations (13)(17) are the full strength properties needed to calibrate the general orthotropic failure criterion (3). They also are of great interest in their own right for an orthotropic laminate. The uniaxial strengths (13)  (16) can also be written in terms of the Poisson s ratios in the compact forms where ν 12 and ν 21 are given by (11) and (12). = ( c 0 +ν 12 c 90 )T tow (18) C 11 = ( c 0 +ν 12 c 90 )C tow (19) T 22 = ( c 90 +ν 21 c 0 )T tow (20) C 22 = ( c 90 +ν 21 c 0 )C tow (21) The basic relations (3) and (13) (17) are powerful results. Not only do they represent the solution to a previously unsolved, very important problem, they do so in an exceedingly simple, clear and concise form. They comprise the orthotropic lamination theory for the strength of fiber dominated composite materials. Contrary to the author s initial and cursory expectation, this much more complex problem and solution is fully as rigorous as the specialized quasiisotropic results in [1]. They include the quasiisotropic forms as a special case. The uniaxial and shear strengths (13) (17) satisfy all the necessary consistency tests. These are as follows. First note that for a unidirectional lamina (13) gives = T tow as must occur. The strengths (13) (17) also have the necessary forms for a fiber dominated crossply laminate necessarily having no shear resistence. The complementary case of only ± 45 s shows the scissoring effect with no resistance
9 that must occur. Finally, when relations (13) (17) are reduced to the quasiisotropic case by taking c 0 = c 90 = c 45 = 1/ 4 the correct quasiisotropic results are recovered from (13) (17), namely (4) and (5). This fiber dominated orthotropic failure theory can be derived for any orthotropic laminate, not just for 0, 90, ± 45 laminates. The forms are a little more complex, but entirely manageable. Such results will be presented in due course. But the 0, 90, ± 45 case is the most important and the simplest case and the one that completely and naturally conforms to orthotropic symmetry. It is emphasized here. The five strengths in (13) (17) are entirely specified by only the two tow strengths for any orthotropic, 0, 90, ± 45 layup. Of course this result is restricted to fiber dominated systems such as carbon fiber, polymeric matrix composites. The enabling operation for this unexpected development is that these five calibrating properties for the orthotropic case are only one dimensional problems. In these cases one can reason which lamina orientations in the four directions are applicable for fiber dominated systems and which are inapplicable for each of the five properties. This operation could not be accomplished if it involved biaxial stress conditions. Effectively critical strain in the 1D fiber direction specifies the failure condition in the uniaxial cases aligned with the symmetry axes. It should be emphasized that fiber dominated systems cannot sustain all stress states. For example for c ±45 = 0 then (13) (15) cannot support a shear stress state. But this simply means that the matrix phase controls failure for such a condition. That would be of no interest for fiber composites. The fiber dominated state must be designed to support the load under all anticipated loading conditions. The final and complete statement of failure criteria for orthotropic laminates is given by the failure criterion (3) with the five calibrating strengths specified by (13) (17) as expressed in terms of the two tow strength properties. To imagine that the complete strength specification for any stress state in the orthotropic laminate could be specified from only two experimental measurements would have seemed impossible before the derivation in this paper.
10 A Specific Example and General Failure Results Everything up to this point up to this point has been motivated and necessitated by original research. Now some interesting consequences from the general theory will be developed and then used in an example. Full blown design procedures for failure would normally involve investigating many different states of stress that could occur in practice. The simplest possible problem of this type will be opened here by prescribing the allowable stress states for the two uniaxial tensile stresses and for the shear stress, taken as individual conditions. After that the more general case will be taken up. As a simple but realistic example take the volume fractions of the lamina orientations as c 0 = 4 7 (22) c 90 = c 45 = 1 7 Thus in terms of volume fractions the anisotropy ratio is c 0 c 90 = 4 (23) From (13) (17) it follows that the tensile uniaxial and shear strengths are given by = T tow T 22 = T tow (24) S 12 = 4 21 T tow C tow 3 With similar forms for C 11 and C 22.
11 From (24) the anisotropy ratio in strengths has the value T 22 = 3 (25) Thus the degree of strength anisotropy is a little less than the anisotropy ratio in the volume fractions (23) but both are highly anisotropic in this example. To go further with a general example take realistic tow strengths for IM7 like carbon fiber polymeric matrix unidirectional strength properties as T tow = 2700 MPa C tow = 1700 MPa (26) For the orthotropic laminate specified by the volume fractions (22) the condition is effectively that of 4/7 of the lamina being in a quasiisotropic arrangement with the additional 3/7 of the lamina added to the 0 direction lamina. The uniaxial and shear strengths are then given by = 1671 MPa C 11 = 1052 T 22 = 557 (27) C 22 = 351 S 12 = 236 The corresponding quasiisotropic problem properties are given by T = 900 MPa C = 567 (28) S = 412
12 Finally the quasiisotropic properties (28) are put into the failure criterion (1) and the orthotropic properties (27) are put into the orthotropic failure criterion (3) giving the resulting failure envelopes shown in Fig. 2, with σ 12 taken as zero. Fig. 2 Failure for fiber dominated unidirectional, intermediate, and quasiisotropic laminates Also shown in Fig. 2 is the representation of the unidirectional tow properties given by (26). Fig. 2 graphically and dramatically shows the progression starting from the unidirectional fiber composites strengths going to and through an intermediate form and finally coming to the other limiting case, the quasiisotropic form. This fiber dominated formalism would not be expected to be realistic near the unidirectional limiting case since it does not include the transverse matrix controlled effects. Other than the need for the micro scale matrix controlled properties the present failure theory applies to and for all orthotropic layup patterns. Complete and comprehensive design applications would involve trade offs between specification of the volume fractions for the four fiber orientations using the lamination rules (13) (17) and then the failure criterion (3). Unsatisfactory
13 results would then require further iteration. Using all this in a numerical program for analysis of an entire structure would complete the process. For this to occur efficiently and effectively it would require a sophisticated numerical algorithm. This new lamination/strength theory provides the vital link in the whole process. With regard to applications and design for applications, it would not be appropriate to use the present fiber dominated methodology for problems having any of the three lamina volume fractions near zero. That condition would require some explicit account of the matrix properties. Also, in any actual application it would always be necessary to have experimental certification of the general results. Further Verification of the Orthotropic Failure Criterion Quasiisotropic laminates are a special case of orthotropic laminates. The previous verification with test results was given in Ref. [1] for the quasiisotropic case. That comparison was for a biaxial spread of data, mainly in the range of compressivecompressive stresses for the principal stresses applied to the laminate. The present verification will involve the state of uniaxial tensile stress at failure. The rationale behind the derivation of the formulas (4) and (5) relating tow failure properties to uniaxial laminate failure properties is as follows. In the tow type failure specimen the strain at failure is given by ε f = T tow E tow (29) where E tow is the elastic modulus of the impregnated tow material. In the quasiisotropic laminate at failure the strain in the lamina that first fails is taken to be the same strain as occurs in the tow specimen. So then for the quasiisotropic laminate in uniaxial tensile stress T E = ε f (30) with E being the laminate elastic modulus. Thus from (29) and (30) T E = T tow E tow (31)
14 Rearranging (31) gives T T tow = E E tow (32) From (32) it follows that if E/E tow = 1/3 can be proven from testing data then it further follows that T/T tow = 1/3 thus verifying (4). Similar arguments would follow for the compressive case of (5). It is much easier and more reliable to measure nondestructive elastic properties than it is to measure failure properties. Thus the proof of E = E tow /3 for the quasiisotropic laminate will suffice to prove (4) and (5). The elastic properties for a quasiisotropic laminate have been quite exhaustively measured by Van Otterloo and Dayal [4]. The values for the elastic modulus E were measured by both ultrasound and mechanical means in 11 different directions in the layup. The mean value for E from the 22 tests was E = 58.5 GPa Measured (33) If only ultrasound data were used the mean was 63.1 GPa. The corresponding modulus of the tow material was measured as E tow = GPa. Using the formula E E tow = 1 3 (34) which is from Ref. [1], Eq. (31), with E 11 = E tow for the fiber dominated system then gives E = 59.5 GPa Predicted (35) Thus the comparison of (33) and (35) provides the further verification of the failure theory.
15 The Next Step The basic research problem of the development of failure theory for fiber composite laminates has now been completed and consummated. This does not however terminate interest in the problem. It actually represents the beginning of a new phase to be used in the applications of fiber composite materials. A major step in that direction will be to develop a complete and comprehensive design methodology for fiber composite laminates. Using the results of this paper, this consolidation will be given in a subsequent paper and it will involve both the stiffness and the strength of fiber composite laminates in a form directly appropriate for applications. References 1. Christensen, R. M., and Lonkar, K., (2017), Failure Theory/Failure Criteria for Fiber Composite Laminates, J. Appl. Mech., 84, Hinton, M. J., and Kaddour, A. S., (2013), The Second WorldWide Failure Exercise Part B, J. Composite Materials, 47, Christensen, R. M., (2014), Completion and Closure on Failure Criteria for Unidirectional Fiber Composite Materials, J. Appl. Mech., 81, Van Otterloo, D. L., and Dayal, V., (2003), How Isotropic are Quasi Isotropic Laminates, Composites Part A: Applied Science and Manufacturing, 34, Richard M. Christensen June 9 th, 2017 Copyright 2017 Richard M. Christensen
QUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationV. FAILURE OF FIBER COMPOSITE LAMINATES PROGRESSIVE
V. FAILURE OF FIBER COMPOSITE LAMINATES PROGRESSIVE DAMAGE AND POLYNOMIAL INVARIANTS Fiber composites are typically used in flat, laminated forms or variations thereof, often also involving woven or braided
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationCoupling of plasticity and damage in glass fibre reinforced polymer composites
EPJ Web of Conferences 6, 48 1) DOI: 1.151/epjconf/1648 c Owned by the authors, published by EDP Sciences, 1 Coupling of plasticity and damage in glass fibre reinforced polymer composites R. Kvale Joki
More informationASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS
ASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS Dieter H. Pahr and Helmut J. Böhm Institute of Lightweight Design and Structural
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationComposite angle ply laminates and netting analysis
10.1098/rspa.2002.1066 FirstCite epublishing Composite angle ply laminates and netting analysis By J. T. Evans and A. G. Gibson School of Mechanical and Systems Engineering, University of Newcastle upon
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationXI. NANOMECHANICS OF GRAPHENE
XI. NANOMECHANICS OF GRAPHENE Carbon is an element of extraordinary properties. The carboncarbon bond possesses large magnitude cohesive strength through its covalent bonds. Elemental carbon appears in
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationBEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS
BEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS Euler S. Dias*, Carlos A. Cimini Jr.* * Federal University of Minas Gerais, Dept. of Structural Engineering, Belo Horizonte 
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationMODELING DYNAMIC FRACTURE AND DAMAGE IN A FIBERREINFORCED COMPOSITE LAMINA WITH PERIDYNAMICS
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Mechanical & Materials Engineering Faculty Publications Mechanical & Materials Engineering, Department of 011 MODELING DYNAMIC
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationGetting Started with Composites Modeling and Analysis
Getting Started with Composites Modeling and Analysis IN THIS WEBINAR: PRESENTED BY: Orthotropic materials and how to define them Composite Laminate properties and modeling Composite failure theories and
More informationVI. CRITICAL EXPERIMENTAL AND THEORETICAL TESTS FOR FAILURE CRITERIA
VI. CRITICAL EXPERIMENTAL AND THEORETICAL TESTS FOR FAILURE CRITERIA The term critical tests implies more than just a routine comparison with some convenient data. First, a candidate failure criterion
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationRELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer
RELATIONSHIP BETWEEN RADIAL COMPRESSIVE MODULUS OF ELASTICITY AND SHEAR MODULUS OF WOOD Jen Y. Liu Research Engineer and Robert J. Ross Supervisory Research Engineer USDA Forest Service Forest Products
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationMechanical Behavior of Composite Tapered Lamina
International Journal of Engineering Research and Development eissn: 2278067X, pissn: 2278800X, www.ijerd.com Volume 10, Issue 8 (August 2014), PP.1927 Mechanical Behavior of Composite Tapered Lamina
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationChapter 5 PlaneStress StressStrain Relations in a Global Coordinate System
Chapter 5 PlaneStress StressStrain Relations in a Global Coordinate System One of the most important characteristics of structures made of fiberreinforced materials, and one which dictates the manner
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationTrace a gamechanging discovery
Trace a gamechanging discovery Stephen W. Tsai Stanford University October 5, 2015 Topics Why trace? The one and only unifying constant Theory of trace simple; easy to understand CPly by Stanford/Chomarat
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationAerospace Structural Composites I Homework 6. Anirban Chaudhuri
Aerospace Structural Composites I Homework 6 Anirban Chaudhuri. The unidirectional Boron/Epoxy layer of Example 6.. (using E = 4GPa, E = 8.5GPa, G = 5.59GPa, =.3, t =.5mm) is to be loaded by combined axial
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More informationEffect of intermediate principal stresses on compressive strength of Phra Wihan sandstone
Rock Mechanics, Fuenkajorn & Phienwej (eds) 211. ISBN 978 974 533 636 Effect of intermediate principal stresses on compressive strength of Phra Wihan sandstone T. Pobwandee & K. Fuenkajorn Geomechanics
More informationMINE ROOF SUPPORT DESIGN AND ANALYSIS. Document no : Revision no : 1.0
MINE ROOF SUPPORT DESIGN AND ANALYSIS Document no : 1806269723 Revision no : 1.0 DOCUMENT TITLE : MINE ROOF SUPPORT DESIGN AND ANALYSIS DOCUMENT NUMBER : 1806269723 ISSUE : Issue 1.0 DATE : 7 October
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationEvaluation of inplane orthotropic elastic constants of paper and paperboard
Evaluation of inplane orthotropic elastic constants of paper and paperboard T. Yokoyama and K. Nakai Department of Mechanical Engineering, Okayama University of Science  Ridaicho, Okayama 75, Japan
More informationA Stress Gradient Failure Theory for Textile Structural Composites. Final Technical Report submitted to ARO
A Stress Gradient Failure Theory for Textile Structural Composites Final Technical Report submitted to ARO By RYAN KARKKAINEN and BHAVANI SANKAR University of Florida Department of Mechanical & Aerospace
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationTensile Properties of ThermoplasticLaminated Composites Based on a Polypropylene Matrix Reinforced with Continuous Twaron Fibers
Tensile Properties of ThermoplasticLaminated Composites Based on a Polypropylene Matrix Reinforced with Continuous Twaron Fibers J. L. MENATUN, P. I. GONZALEZCHI Centro de Investigación Científica de
More informationINITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS INITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES E. Iarve 1,2*, D. Mollenhauer 1, T. Breitzman 1, K. Hoos 2, M. Swindeman 2 1
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationChapter 6: Plastic Theory
OHP Mechanical Properties of Materials Chapter 6: Plastic Theory Prof. Wenjea J. Tseng 曾文甲 Department of Materials Engineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W. F.
More informationModelling of multiaxial ultimate elastic wall stress (UEWS) test for glass fibre reinforced epoxy (GRE) composite pipes
pplied Mechanics and Materials Vol. 367 (013) pp 113117 Online available since 013/ug/16 at www.scientific.net (013) Trans Tech Publications, Switzerland doi:10.408/www.scientific.net/mm.367.113 Modelling
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationPractice Final Examination. Please initial the statement below to show that you have read it
EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationBending Load & Calibration Module
Bending Load & Calibration Module Objectives After completing this module, students shall be able to: 1) Conduct laboratory work to validate beam bending stress equations. 2) Develop an understanding of
More information15 INTERLAMINAR STRESSES
15 INTERLAMINAR STRESSES 151 OUTOFPLANE STRESSES Classical laminate plate theor predicts the stresses in the plane of the lamina,, and τ but does not account for outofplane stresses, τ and τ. It assumes
More informationA New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms
A New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms DARUN BARAZANCHY 1, WILLIAM ROTH 2 and VICTOR GIURGIUTIU 3 ABSTRACT Dispersion curve algorithms
More informationCrashworthiness of composite structures: Experiment and Simulation
Crashworthiness of composite structures: Experiment and Simulation Francesco Deleo, Bonnie Wade and Prof. Paolo Feraboli (UW) Dr. Mostafa Rassaian (Boeing R&T) JAMS 2010 The Joint Advanced Materials and
More informationLAMINATE DESIGN WITH NONSTANDARD PLY ANGLES FOR OPTIMISED INPLANE PERFORMANCE
21 st International Conference on Composite Materials Xi an, 2025 th August 2017 LAMINATE DESIGN WITH NONSTANDARD PLY ANGLES FOR OPTIMISED INPLANE PERFORMANCE Mark W.D. Nielsen 1, Kevin J. Johnson 1,
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationMechanics of Biomaterials
Mechanics of Biomaterials Lecture 7 Presented by Andrian Sue AMME498/998 Semester, 206 The University of Sydney Slide Mechanics Models The University of Sydney Slide 2 Last Week Using motion to find forces
More informationFRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
Proc. 2 nd ESIS TC4 Conference on Polymers and Composites, in press, 1999 Author prepared reprint FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
More information